| Composition    | Minimum load to generate cracks (N) | Minimum load to generate cracks (N) | Minimum load to generate cracks (N) | Minimum load to generate cracks (N) | Maximum load (N) |
| Na2O-TiO2-SiO2 | 4 Cracks                            | 3 Cracks                            | 2 Cracks                            | 1 Crack                             | 0 Cracks         |
| 10-4-86        | 4.6                                 | 2.8                                 | 1.6                                 | 0.8                                 | 0.54             |
| 10-7-83        | 10.5                                | 6.3                                 | 3.2                                 | 1.4                                 | 0.76             |
| 10-10-80       | 5.7                                 | 3.4                                 | 1.8                                 | 0.84                                | 0.51             |
| 15-4-81        | 14.7                                | 4.3                                 | 2.9                                 | 1.0                                 | 0.50             |
| 15-7-78        | 2.9                                 | 1.8                                 | 1.1                                 | 0.65                                | 0.50             |
| 15-10-75       | 1.1                                 | 0.9                                 | 0.75                                | 0.60                                | 0.44             |
| 20-4-76        | 1.2                                 | 1.0                                 | 0.81                                | 0.61                                | 0.42             |
| 20-7-73        | 2.9                                 | 1.2                                 | 0.50                                | 0.20                                | 0.08             |
| 20-10-70       | 2.9                                 | 2.1                                 | 1.4                                 | 0.74                                | 0.15             |
| 25-4-71        | 9.8                                 | 7.2                                 | 5.1                                 | 3.5                                 | 2.6              |
| 25-7-68        | 2.9                                 | 2.5                                 | 2.0                                 | 1.5                                 | 1.0              |
| 25-10-65       | 9.8                                 | 6.7                                 | 4.5                                 | 3.3                                 | 2.9              |

Caption: The minimum load required to generate a given number of cracks around a Vickers indent for Na2O-TiO2-SiO2 glasses. The zero cracks column represents the maximum load at which no cracks could be detected (SEM and Optical microscope) at the corners of a Vickers indent.

You are provided with a table from a material science paper. Here are JSON templates for two types of numeric cells: "Other" and "Glass_Compound_Amount":
{"value": "xx", "type": "Other"}
{"value": "xx", "type": "Glass_Compound_Amount", "constituent": "xx", "unit": "xx", "material": "xx"}

Please describe all numeric cells in the above table following the JSON templates (proceeding by row in a left-right, top-down direction). For each cell, output one JSON description per line. For any unanswerable attributes in the templates, set their value to the placeholder "xx".

Cell Description:
{"value": "10", "type": "Glass_Compound_Amount", "constituent": "Na2O", "unit": "mol", "material": "xx"}
{"value": "4", "type": "Glass_Compound_Amount", "constituent": "TiO2", "unit": "mol", "material": "xx"}
{"value": "86", "type": "Glass_Compound_Amount", "constituent": "SiO2", "unit": "mol", "material": "xx"}
{"value": "4.6", "type": "Other"}
{"value": "2.8", "type": "Other"}
{"value": "1.6", "type": "Other"}
{"value": "0.8", "type": "Other"}
{"value": "0.54", "type": "Other"}
{"value": "10", "type": "Glass_Compound_Amount", "constituent": "Na2O", "unit": "mol", "material": "xx"}
{"value": "7", "type": "Glass_Compound_Amount", "constituent": "TiO2", "unit": "mol", "material": "xx"}
{"value": "83", "type": "Glass_Compound_Amount", "constituent": "SiO2", "unit": "mol", "material": "xx"}
{"value": "10.5", "type": "Other"}
{"value": "6.3", "type": "Other"}
{"value": "3.2", "type": "Other"}
{"value": "1.4", "type": "Other"}
{"value": "0.76", "type": "Other"}
{"value": "10", "type": "Glass_Compound_Amount", "constituent": "Na2O", "unit": "mol", "material": "xx"}
{"value": "10", "type": "Glass_Compound_Amount", "constituent": "TiO2", "unit": "mol", "material": "xx"}
{"value": "80", "type": "Glass_Compound_Amount", "constituent": "SiO2", "unit": "mol", "material": "xx"}
{"value": "5.7", "type": "Other"}
{"value": "3.4", "type": "Other"}
{"value": "1.8", "type": "Other"}
{"value": "0.84", "type": "Other"}
{"value": "0.51", "type": "Other"}
{"value": "15", "type": "Glass_Compound_Amount", "constituent": "Na2O", "unit": "mol", "material": "xx"}
{"value": "4", "type": "Glass_Compound_Amount", "constituent": "TiO2", "unit": "mol", "material": "xx"}
{"value": "81", "type": "Glass_Compound_Amount", "constituent": "SiO2", "unit": "mol", "material": "xx"}
{"value": "14.7", "type": "Other"}
{"value": "4.3", "type": "Other"}
{"value": "2.9", "type": "Other"}
{"value": "1.0", "type": "Other"}
{"value": "0.50", "type": "Other"}
{"value": "15", "type": "Glass_Compound_Amount", "constituent": "Na2O", "unit": "mol", "material": "xx"}
{"value": "7", "type": "Glass_Compound_Amount", "constituent": "TiO2", "unit": "mol", "material": "xx"}
{"value": "78", "type": "Glass_Compound_Amount", "constituent": "SiO2", "unit": "mol", "material": "xx"}
{"value": "2.9", "type": "Other"}
{"value": "1.8", "type": "Other"}
{"value": "1.1", "type": "Other"}
{"value": "0.65", "type": "Other"}
{"value": "0.50", "type": "Other"}
{"value": "15", "type": "Glass_Compound_Amount", "constituent": "Na2O", "unit": "mol", "material": "xx"}
{"value": "10", "type": "Glass_Compound_Amount", "constituent": "TiO2", "unit": "mol", "material": "xx"}
{"value": "75", "type": "Glass_Compound_Amount", "constituent": "SiO2", "unit": "mol", "material": "xx"}
{"value": "1.1", "type": "Other"}
{"value": "0.9", "type": "Other"}
{"value": "0.75", "type": "Other"}
{"value": "0.60", "type": "Other"}
{"value": "0.44", "type": "Other"}
{"value": "20", "type": "Glass_Compound_Amount", "constituent": "Na2O", "unit": "mol", "material": "xx"}
{"value": "4", "type": "Glass_Compound_Amount", "constituent": "TiO2", "unit": "mol", "material": "xx"}
{"value": "76", "type": "Glass_Compound_Amount", "constituent": "SiO2", "unit": "mol", "material": "xx"}
{"value": "1.2", "type": "Other"}
{"value": "1.0", "type": "Other"}
{"value": "0.81", "type": "Other"}
{"value": "0.61", "type": "Other"}
{"value": "0.42", "type": "Other"}
{"value": "20", "type": "Glass_Compound_Amount", "constituent": "Na2O", "unit": "mol", "material": "xx"}
{"value": "7", "type": "Glass_Compound_Amount", "constituent": "TiO2", "unit": "mol", "material": "xx"}
{"value": "73", "type": "Glass_Compound_Amount", "constituent": "SiO2", "unit": "mol", "material": "xx"}
{"value": "2.9", "type": "Other"}
{"value": "1.2", "type": "Other"}
{"value": "0.50", "type": "Other"}
{"value": "0.20", "type": "Other"}
{"value": "0.08", "type": "Other"}
{"value": "20", "type": "Glass_Compound_Amount", "constituent": "Na2O", "unit": "mol", "material": "xx"}
{"value": "10", "type": "Glass_Compound_Amount", "constituent": "TiO2", "unit": "mol", "material": "xx"}
{"value": "70", "type": "Glass_Compound_Amount", "constituent": "SiO2", "unit": "mol", "material": "xx"}
{"value": "2.9", "type": "Other"}
{"value": "2.1", "type": "Other"}
{"value": "1.4", "type": "Other"}
{"value": "0.74", "type": "Other"}
{"value": "0.15", "type": "Other"}
{"value": "25", "type": "Glass_Compound_Amount", "constituent": "Na2O", "unit": "mol", "material": "xx"}
{"value": "4", "type": "Glass_Compound_Amount", "constituent": "TiO2", "unit": "mol", "material": "xx"}
{"value": "71", "type": "Glass_Compound_Amount", "constituent": "SiO2", "unit": "mol", "material": "xx"}
{"value": "9.8", "type": "Other"}
{"value": "7.2", "type": "Other"}
{"value": "5.1", "type": "Other"}
{"value": "3.5", "type": "Other"}
{"value": "2.6", "type": "Other"}
{"value": "25", "type": "Glass_Compound_Amount", "constituent": "Na2O", "unit": "mol", "material": "xx"}
{"value": "7", "type": "Glass_Compound_Amount", "constituent": "TiO2", "unit": "mol", "material": "xx"}
{"value": "68", "type": "Glass_Compound_Amount", "constituent": "SiO2", "unit": "mol", "material": "xx"}
{"value": "2.9", "type": "Other"}
{"value": "2.5", "type": "Other"}
{"value": "2.0", "type": "Other"}
{"value": "1.5", "type": "Other"}
{"value": "1.0", "type": "Other"}
{"value": "25", "type": "Glass_Compound_Amount", "constituent": "Na2O", "unit": "mol", "material": "xx"}
{"value": "10", "type": "Glass_Compound_Amount", "constituent": "TiO2", "unit": "mol", "material": "xx"}
{"value": "65", "type": "Glass_Compound_Amount", "constituent": "SiO2", "unit": "mol", "material": "xx"}
{"value": "9.8", "type": "Other"}
{"value": "6.7", "type": "Other"}
{"value": "4.5", "type": "Other"}
{"value": "3.3", "type": "Other"}
{"value": "2.9", "type": "Other"}